SlideShare
Explore
Search
You
Upload
Login
Signup
Home
Technology
Education
More Topics
For Uploaders
Collect Leads
Get Started
Tips & Tricks
Tools
For Business
Constructing a mathematical models to predict compressive strength of conc
Upcoming SlideShare
Loading in...
5
×
1
1
of
20
Like this document? Why not share!
Share
Email
Boc Lecture 3 the multistep nature ...
by Karobi Moitra MS,...
2035 views
05.12.09(b): Energy Balance and Obe...
by Open.Michigan
457 views
Does a Virus Cause Breast Cancer?
by Vera Gruessner
426 views
House mouse
by wahabhse
8 views
Share SlideShare
Facebook
Twitter
LinkedIn
Google+
Email
Email sent successfully!
Embed
Size (px)
Start on
Show related SlideShares at end
WordPress Shortcode
Link
Constructing a mathematical models to predict compressive strength of conc
885
Share
Like
Download
iaeme
Follow
0
0
0
0
Published on
Jul 19, 2013
Published in:
Business
,
Technology
0 Comments
0 Likes
Statistics
Notes
Full Name
Comment goes here.
12 hours ago
Delete
Reply
Spam
Block
Are you sure you want to
Yes
No
Your message goes here
Post
Be the first to comment
Be the first to like this
No Downloads
Views
Total Views
885
On Slideshare
0
From Embeds
0
Number of Embeds
0
Actions
Shares
0
Downloads
32
Comments
0
Likes
0
Embeds
0
No embeds
No notes for slide
Constructing a mathematical models to predict compressive strength of conc
1. International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 1 CONSTRUCTING A MATHEMATICAL MODELS TO PREDICT COMPRESSIVE STRENGTH OF CONCRETE FROM NON-DESTRUCTIVE TESTING Abbas S. Al-Ameeri 1 K.A.AL- Hussain 2 M.S Essa3 1 (Civil, Engineering/ University of Babylon, Babylon City, Iraq) 2 (Civil, Engineering/University of Babylon, Al-Najaf City, Iraq) 3(Civil, Engineering/ University of Babylon, Babylon City, Iraq) ABSTRACT Nondestructive tests NDT are considered as a one of the methods of evaluation and quality control of concrete. The fundamental aim of the present study is constructing a mathematical model to predict comp. of concrete from Nondestructive testing, in addition the study of (NSC and HSC) properties (density, compressive strength (20-100) Mpa,) using NDT methods namely; Schmidt Hammer test (RN )and Ultrasonic Pulse Velocity test ( UPV) with destructive test methods at different four ages (7, 28, 56 and 90) days. This study used ready mixes (1:2:4 and 1:1.5:3) and design mixes (C40, C50, C60, C70, C80, C90 and C100), in order to find the relationship between comp. of concrete with (RN and UPV), and comp. of concrete-combined NDT(RN and UPV) relationship, for all mixes (as freelance and as group). The results of compressive strength for both types of concrete NSC and HSC exhibit an increase with the increase of bulk density and time of curing. Also, the results show a good correlation between compressive strength and (RN) and the relationship between the two is not affected by maximum aggregate size (MAS). Also, a good correlation between compressive strength and Ultrasonic Pulse Velocity (UPV) and The value of UPV in HSC increased 8% from 28 days to 90 days. Also, The results indicate that the percentage of increase in direct method to surfacing method of UPV for (7, 28, 56 and 90) days is (7%, 5%, 4% and 3.5%) respectively, due to the higher the continuity of hydration of cement. Also, the pulse velocity of concrete is decreased by increasing the cement paste, especially for concrete with high w/c. Keywords: Nondestructive tests, Schmidt hammer test(RN), Ultrasonic pulse velocity test (UPV) , Density , Compressive strength I. INTRODUCTION The concrete is a composite material that consists essentially of a binding medium within which are embedded particles or fragments of aggregate. In hydraulic cement concrete the binder is INTERNATIONAL JOURNAL OF CIVIL ENGINEERING AND TECHNOLOGY (IJCIET) ISSN 0976 – 6308 (Print) ISSN 0976 – 6316(Online) Volume 4, Issue 4, July-August (2013), pp. 01-20 © IAEME: www.iaeme.com/ijciet.asp Journal Impact Factor (2013): 5.3277 (Calculated by GISI) www.jifactor.com IJCIET © IAEME
2.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 2 formed from a mixture of hydraulic cement and water[1],Concrete composites of (Cement ,Aggregates , Water and Admixtures ). Normal strength concrete NSC is defined by American Concrete Institute (ACI committee 211.1 -02) [2] as “concrete that has a specified average compressive strength of 40 MPa or less at 28 days” but should be not less than 17 Mpa (ACI committee 318M-05) [3] and the high strength concrete HSC is defined by American Concrete Institute (ACI committee 363R-97) [4] as “concrete that has a specified average compressive strength of 41MPa or more at 28 days. The Mix proportions for HSC are influenced by many factors, including specified performance properties, locally available materials, local experience, personal preferences and cost [5]. HSC mix proportioning is a more critical process than the design of normal strength concrete mixtures (ACI Committee 363R-97) [4]. When developing mixture proportions for HSC, three fundamental factors must be considered in order to produce a mix design satisfying its intended property requirements (mechanical properties of the aggregates; mechanical properties of the paste and Bond strength at the paste-aggregate interfacial transition zone) [6], [7] . For many years in concrete practice, the most widely used test for concrete has been the compression test of the standard specimens (cube or cylinder) . It is often necessary to test concrete structures after the concrete has hardened to determine whether the structure is suitable for its designed use. Ideally such testing should be done without damaging the concrete [8] . The tests available for testing concrete range from the completely non-destructive, where there is no damage to the concrete, through those where the concrete surface is slightly damaged, to partially destructive tests, such as core tests and pullout and pull off tests, where the surface has to be repaired after the testing. The range of properties that can be assessed using Non- destructive tests and partially destructive tests. Nondestructive test define as the test which either do not alter the concrete or result in superficial local damage [9], [8] . Non-destructive testing can be applied to both old and new structures. For new structures, the principal applications are likely to be for quality control or the resolution of doubts about the quality of materials or construction. The testing of existing structures is usually related to an assessment of structural integrity or adequacy [10] . In addition, in-situ NDT was introduced to supply the engineer with information on one or more of the following properties of the structural material: in-situ strength properties, durability, density, moisture content, elastic properties, extent of visible cracks, thickness of structural members having one face exposed, position of the steel reinforcement and concrete cover over the reinforcement. Most emphasis has been placed on the determination of in-situ strength and durability [11] . Non-destructive tests and partially destructive tests is quite large and includes such fundamental parameters as density, elastic modulus and strength as well as surface hardness and surface absorption, and reinforcement location, size and distance from the surface. In some cases it is also possible to check the quality of workmanship and structural integrity by the ability to detect voids, cracking and delaminating [10]one of types of Non-destructive test methods is Schmidt hammer test, In 1940S ERNst Schmidt, a Swiss engineer, developed a device for testing concrete based upon the rebound principle, This device consists of the following main components outer body, plunger, hammer, and spring. To perform the test, the plunger retracts against a spring when pressed against the concrete surface and this spring is automatically released when fully tensioned, causing the hummer mass to impact against the concrete through the plunger. The rebounding hammer moves the slide indicator, which records the rebound distance. The rebound distance is measured on a scale numbered from (10 to 100) and is recorded as the rebound number indicated on the scale [12], [13] . There are Factors influencing of the rebound test results, mix characteristics (cement type, cement content and coarse aggregate type) and member characteristic (mass, compaction, surface
3.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 3 type, age, surface carbonation, moisture condition and stress state and temperature). The strength- rebound number relationship is depended on many factors that are influence on test results which may empirically affect the relationship between compressive strength and rebound number. Practically, it is agreed that there is no unique relationship between concrete strength and rebound number. Many investigations have been done to obtain a relationship between rebound number and compressive strength, locally (Raouf and Samurai-99) [14] obtained an experimental relationship to estimate concrete compressive strength using rebound number f cu=0.74 RN 1.12 ……… (I-1) Where: fcu: Concrete compressive strength in MPa. (cube) , RN: rebound number. (Hussam -08) [11] obtained a mathematical relationship between concrete compressive strength (fcu:) and rebound number (RN), as follows: f cu=- 65.33+2.38 RN ……… (I-2) Where: fcu: Concrete compressive strength in Mpa. (cube), RN: Rebound number. Another method of Nondestructive test is ultrasonic pulse velocity test( UPV).The UPV method is a stress wave propagation method that involves measuring the travel time, over a known path length, of ultrasonic pulse waves. The pulses are introduced into the concrete by a piezoelectric transducer and a similar transducer acts as receiver to monitor the surface vibration caused by the arrival of the pulse. A timing circuit(t) is used to measure the time it takes for the pulse to travel from the transmitting to the receiving transducers during the materials path (L). The pulse velocity (V) is given by dividing path length (L) over transit time (t) V=L / T ……… (I-3) The presence of low density or cracked concrete increases the travel time which results in a lower pulse velocity. The factors affecting on strength-pulse velocity relationship water/cement ratio (w/c), aggregate size, grading, type, and content ,the concrete age, moisture condition, compaction ,curing temperature, path length, level of stress [13] . In estimation, the strength of in-situ the concrete strength from pulse velocity measurements, an empirical relationship must be established on test specimens in the laboratory. In practice, it is generally agreed that there is no unique relationship between concrete strength and UPV. There exist factors which may affect one parameter only leading to existence of different relationships. Locally (Raouf and Samurai-99)[14] obtained an experimental relationship to estimate concrete compressive strength using rebound number. fcu= 2.8 e 0.58V ……… (I-4) Where: fcu: Concrete compressive strength in Mpa. (cube) , V: UPV in (km/sec) (Hussam-08)[11] obtained a mathematical relationship between concrete compressive strength (fcu) in Mpa and ultrasonic pulse velocity UPV, as follows: fcu= 0.086 e 1.58V ……… (I-5) Where: fcu in (Mpa) and V: UPV in (km/sec).
4.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 4 In many time used combined nondestructive test methods to estimate concrete strength. By combining results from more than one NDT test, a multivariable correlation can be established to estimate strength. Combined methods are reported to increase the reliability of the estimated strength. The underlying concept is that if the two methods are influenced in different ways by the same factor, their combined use results in a canceling effect that improves the accuracy of the estimated strength. For example, an increase in moisture content increases pulse velocity but decreases the rebound number. Locally (Raouf and Samurai -99)[14] obtained an experimental relationship to estimate concrete compressive strength using combined rebound number and ultrasonic pulse velocity at different ages (28, 60 and 90) days and by using statistical analysis methods, the following relation was obtained: fcu =0.93RN 0.63 e 0.31V ………..(I-6) Where: fcu : in MPa , RN: Rebound number, V : UPV in (km/sec). (Hussam -08)[11] obtained an experimental relationship to estimate compressive strength of concrete using combined rebound number and ultrasonic pulse velocity. By method of multiple linear regression analysis using (statistica-6.0) computer program, the following relation was obtained: fcu =0.0031RN 1.65 V 2.075 ………..(I-7) Where: fcu in (MPa), RN: Rebound number, V: UPV in (km/sec). II. EXPERIMENTAL WORKS This paragraph includes detailed information about description of material and mixes, mixing procedure, casting and curing and testing are carried out on sample to achieve the aim of this study. A. Materials NSC and HSC are obtained by selecting suitable materials, good quality control and proportioning. The material must be conforming to (ACI committee 211.1-2002) [2] and (ACI committee 363R, 1997)[4] requirements. 1. Cement Ordinary Portland cement (OPC) (type I) was used in this study. The cement was produced by United Cement Company “UCC” commercially known as “Tasluja” produced in Al-Sulaymaniyah City. The Table I shows physical properties and chemical analysis of this cement, which comply with the (I.Q.S. No.5 -84) requirements [15] . 2. Fine Aggregate (F.A) Natural siliceous sand brought from (Al-Ukhaider) region was used in this study. the results showed that the grading and sulfate content conformed to the (I.Q.S. No.45 -84 Zone2) [16] as illustrated in Table II. 3. Coare Aggregate (C.A) Coarse aggregate used in this study was cleaned, cubical, and 100% crushed gravel from (Al- Niba’ee) region with two maximum size are used (14 , 20) mm. The Table III shows the grading of the aggregate with size (14mm) , (20mm) respectively, the results were conformed to the (I.Q.S. No.45-84) [16] .
5.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 5 4. Silica fume (SF) Silica fume used in this study was Turkey production , The physical properties and chemical composition of SF used are shown in Table IV, it was conformed to the chemical and physical requirements of (ASTM C1240 - 03) [17] . TABLE I CHEMICAL AND PHYSICAL PROPERTIES OF CEMENT Oxide composition Abbreviation Content % IQS No.5/1984 Limits Calcium oxide CaO 62.20 - Silicon oxide SiO2 20.39 - Aluminum oxide Al2O3 4.55 - Ferric oxide Fe2O3 3.81 - Magnesium oxide MgO 2.36 ≤ 5.0% Sulphur trioxide SO3 1.97 ≤ 2.8% Loss on Ignition L.O.I 2.41 ≤ 4.0% Insoluble residue I.R 1.11 ≤ 1.5% Lime saturation factor L.S.F 0.93 0.66-1.02 Free lime F.L 0.26 - Main Compounds according to (Bogue’s equations) Tricalcium Silicate C3S 56.55 - Dicalcium Silicate C2S 15.88 - Tricalcium Aluminate C3A 5.61 - Tetracalcium Alumino-Ferrite C4AF 11.58 - Physical properties Test results IQS No.5/1984 Limits Specific surface area (Fineness) (Blaine method), m2/kg 310 ≥ 230 Soundness (Auto clave), % 0.23 ≤ 0.8 Setting time (Vicat’s apparatus) Initial setting time, min. Final setting time, hrs: min. 90 4:15 ≥ 45 min ≤ 10 hrs Compressive strength of mortar at : Age - 3days, MPa Age - 7days, MPa 23 30 ≥ 15 ≥ 23
6.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 6 TABLE II PROPERTIES OF FINE AGGREGATE Sieve size (mm) percentage passing IQS No.45/1984 Limits, Zone 2 ASTM C33-03 Limits 10.0 100 100 100 4.75 99 90-100 95-100 2.36 90 75-100 80-100 1.18 81 55-90 50-85 0.60 52 35-59 25-60 0.30 25 8-30 5-30 0.15 6 0-10 0-10 Physical properties Test results IQS No. 45/1984 Limits Specific gravity 2.67 - Sulfate content (SO3) % 0.30 ≤ 0.5 Absorption % 1.5 - Fineness modulus 2.48 - dry-rodded unit weight(kg/m3 ) 1750 - TABLE III PROPERTIES OF COARSE AGGREGATE Sieve Size (mm) Percentage Passing IQS 45-84 limits Size 5-14 Size 5-20 Size 5-14 Size 5-20 37.5 - 100 - - 25 - 100 - 100 20 100 100 100 95-100 14 100 - 90-100 - 10 60 42 50-85 30-60 5 5 5 0-10 0-10 2.36 0 0 - - Physical properties Test results IQS No. 45/1984 Limits MAS (14)mm MAS (20)mm Specific gravity 2.65 2.62 - Sulfate content (SO3) % 0.08 0.08 ≤ 0.1 DRUW (kg/m3) 1650 1641 - 5. Superplasticizer (SP) To produce HSC with silica fume a high range water reducer was used. It was based on polycarboxylic ether and had the trade mark “Glenium 51”. It was complied with (IQS No.1431- 89)[18] and (ASTM C494-05)[19] type F, Table V shows the typical properties of Glenium 51.
7.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 7 TABLE IV PHYSICAL AND CHEMICAL PROPERTIES OF SILICA FUME ** Physical property SF Specific surface area , ( m2/ kg) * 25000 Bulk density ( kg / m³ ) 480 Specific gravity 2.2 Color Gray powder Chemical property Oxides Content (%) Requirement of ASTM C1240-05 SiO2 95.68 ≥ 85 Al2O3 0.5 – Fe2O3 – – Na2O – – CaO 1.30 – MgO 0.43 – SO3 0.31 ≤ 4 SiO2 95.68 ≥ 85 * The specific surface area estimated using the nitrogen adsorption method ** Physical properties are according to manufacturer TABLE V TECHNICAL PROPERTIES OF THE GLENIUM 51# Technical description Properties Appearance Viscous liquid Color Light brown Relative density 1.1 @ 20 oC Transport Not classify as dangerous pH value 6.6 Labeling No hazard label required Dosage* 0.5-1.6 liters per 100 kg of cement Viscosity 128 ± 30 CPS @ 20 o C * Dosages outside this range are permissible with trial mixes. # Properties from product catalogue 6. Water Tap water was used for both mixing and curing of concrete in this work. B. Concrete mixes In order to achieve the scopes of this study, the work is divided into fifteen sets of concrete mixes, divided into two sets (ready mixes and design mixes). Mix design for normal strength concrete was made using MAS (20) mm using (ACI committee 211.1-02)[2] method , the details of the two mix groups are shown in Table VI.
8.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 8 TABLE VI PROPORTION OF FIRST SET OF MIXTURES Mix symbol The mix proportion by Vol. The mix proportion by weight w/c Slump (mm) A1 1:2:4 (1:2.5:4.63) 0.60 5 A2 1:2:4 (1:2.5:4.63) 0.576 10 A3 1:2:4 (1:2.5:4.63) 0.55 15 A4 1:2:4 (1:2.5:4.63) 0.525 20 B1 1:1.5:3 (1:1.91:3.5) 0.45 5 B2 1:1.5:3 (1:1.91:3.5) 0.427 10 B3 1:1.5:3 (1:1.91:3.5) 0.40 15 B4 1:1.5:3 (1:1.91:3.5) 0.375 20 C40 1:0.97:1.8 (1:1.17:2.2) 0.42 75-100 C50 1:0.88:1.68 (1:1.1:2.02) 0.38 75-100 Mix design for high strength concrete was depended on replacement SF (15) % by weight of cement were used, and using (ACI committee 211.4R)[20] and (ACI committee 211.1R)[21] to choose air content reduced by one percent by (Holland -05)method [22] . The initial dosages of superplasticizer depending on slump test result [23] . The MAS of coarse aggregate was used (14mm), the Table VII shows the proportion of mixes of high strength concrete . TABLE VII THE PROPORTION OF SECOND SET OF MIXTURES Mix Symbol The mix proportion by weight Cement kg/m3 SF kg/m3 HRWR % wt of cementitious w/c+p Slump (mm) C60 1:1.07:2.03 527 --- 0.08 0.36 75-100 C70 1:1.04:1.97 543 --- 0.29 0.33 75-100 C80 1:0.96:1.82 585 --- 0.55 0.3 75-100 C90 1:1.24:2.13 468 70 1.9 0.24 75-100 C100 1:1.28:2.20 442 78 2.4 0.22 75-100 C. Casting and curing of test specimens The molds used were cleaned, assembled and oiled. The concrete was cast in molds in three layers; each layer compacted by using vibrating Table for adequate time to remove any entrapped air. In the second day the specimens were demolded and put in water for curing at temperature (24+ 3) ◦ C until the day of testing . D. Testing fresh and harden concrete 1. Slump test This test is used to determine the workability of concrete mixture according to (I.Q.S. No.354 -90) [24] by using standard slump cone. 2. Schmidt hammer test This test has been done according to (I.Q.S. No.325 -93)[25] on cubic specimens of (150 , 100) mm for NSC and HSC respectively, edges which have been fixed by applying 7 MPa in a compression machine to avoid any movement during this test
9.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue 3. Ultrasonic pulse velocity test This test has been done according to (I.Q.S. No.300 (150,100) mm for NSC and HSC respectively, using transducers with frequency 54 kHz, 4. Compressive Strength Standard cubes (150) mm for NSC and (100) mm for HSC are used according to (I.Q.S. No.284 -91)[27]. The machine which used in the tests was one of the electronic type of capacity with (15 N/mm2 /minute) applied III. RESULTS AND DISCUSSION Both tests of Schmidt hammer rebound number and Ultrasonic pulse velocity are carried out simultaneously on the same cubes of (150 and 100) mm for NSC carried out at (7, 28, 56 and 90) days. A. The relationship between density a The density considered the measurement to describe the properties of concrete, increasing the density of concrete produce increasing in the surface hard increasing in value of rebound number, and through the concrete, and consequently increase in velocity of ultrasonic wave produce high strength of concrete, because decreasing the pores due to using crushed aggregate, high content of cement and SF. The relationship between density and (rebound number presented in Fig.1, 2 respectively for all mixes Fig. 1 Relationship between Density and 2250 2300 2350 2400 2450 2500 15 25 Density-kg/m3 28-day 90-day International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 9 This test has been done according to (I.Q.S. No.300 -91)[26] on cubic specimens of (150,100) mm for NSC and HSC respectively, using transducers with frequency 54 kHz, 50) mm for NSC and (100) mm for HSC are used according to (I.Q.S. which used in the tests was one of the electronic type of /minute) applied load rate. DISCUSSION s of Schmidt hammer rebound number and Ultrasonic pulse velocity are carried out simultaneously on the same cubes of (150 and 100) mm for NSC and HSC respectively. All tests are carried out at (7, 28, 56 and 90) days. The relationship between density and (RN and UPV) The density considered the measurement to describe the properties of concrete, increasing the density of concrete produce increasing in the surface hardness of concrete, as the result in value of rebound number, and decrease the time of transference ultrasonic the concrete, and consequently increase in velocity of ultrasonic wave produce high strength of concrete, because decreasing the pores due to using crushed aggregate, high content of cement and The relationship between density and (rebound number and Ultrasonic Pulse Velocity) is 2 respectively for all mixes as group the strength from (20-100) M Fig. 1 Relationship between Density and RN at (28-90) days D = 162.41ln(RN) + 1796 R² = 0.9861 D = 172.72ln(RN) + 1747 R² = 0.9939 35 45 55 65 Rebound number International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (2013), © IAEME on cubic specimens of (150,100) mm for NSC and HSC respectively, using transducers with frequency 54 kHz, 50) mm for NSC and (100) mm for HSC are used according to (I.Q.S. which used in the tests was one of the electronic type of 2000 kN s of Schmidt hammer rebound number and Ultrasonic pulse velocity are carried out HSC respectively. All tests are The density considered the measurement to describe the properties of concrete, increasing the ness of concrete, as the result caused decrease the time of transference ultrasonic wave the concrete, and consequently increase in velocity of ultrasonic wave produce high strength of concrete, because decreasing the pores due to using crushed aggregate, high content of cement and Ultrasonic Pulse Velocity) is 100) MPa. 1796.5 1747 75
10.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue Fig. 2 Relationship between Density and (UPV) at (28 B. The Relationship between Compressive Strength and The results show that the relationship between compressive strength and rebound number is different from mix to other because the difference in properties of the mixes and (w/c) ratio. Also, the results show large similarity behavior of the mix (A1, A2, A3 and A4) and (B1, B2, B3 and B4) because it is ready mix and normal strength and show similarity behavior of the mix (C40, C50 and C60), and show similarity behavior of the mix(C70, C80, C90 and C100), as shown in Fig.3. Fig. 3 the relationship between Compressive strength 1:1.5:3, (C40, C 0 10 20 30 40 50 60 70 80 90 100 110 15 25 Compressivestrength-MPa 1:2.5:4.63 2250 2300 2350 2400 2450 2500 3.25 3.65 Density-kg/m3 28-day 90-day International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 10 Fig. 2 Relationship between Density and (UPV) at (28-90) days Relationship between Compressive Strength and RN The results show that the relationship between compressive strength and rebound number is ause the difference in properties of the mixes and (w/c) ratio. Also, the results show large similarity behavior of the mix (A1, A2, A3 and A4) and (B1, B2, B3 and B4) because it is ready mix and normal strength and just difference is the changing in (w/ similarity behavior of the mix (C40, C50 and C60), and show similarity behavior of the mix(C70, C80, C90 and C100), as shown in Fig.3. Fig. 3 the relationship between Compressive strength-RN at all ages for the , C50, C60) and (C70, C80, C90, C100) at all ages fcu = 2.8789RN - fcu = 3.6298RN - fcu = 3.3032RN - fcu = 2.7833RN - 35 45 55 65 Rebound number 1:1.91:3.5 D = 134.98V + 1814 R² = 0.9287 D = 159.45V + 1680 R² = 0.8751 4.05 4.45 4.85 Ultrasonic pulse velocity-km/sec International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (2013), © IAEME The results show that the relationship between compressive strength and rebound number is ause the difference in properties of the mixes and (w/c) ratio. Also, the results show large similarity behavior of the mix (A1, A2, A3 and A4) and (B1, B2, B3 and B4) just difference is the changing in (w/c) ratio, and similarity behavior of the mix (C40, C50 and C60), and show similarity behavior of the mixes(1:2:4, - 47.03 - 83.197 - 82.797 - 74.533 75 1814.8 9287 1680.1 8751 5.25
11.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue The Fig. 3 shows that the value of it because the increasing coarse aggregate and concrete homogeneity, and this properties caused increasing hardness of concrete. The Fig. 4 shows the relationship between compressive strength of concrete and RN for the all mixes at all ages. After using statistical analyses by (SPSS.19) program, it could be found that the linear expressions are giving higher coefficient of correlation than other expressions, the expression obtained from Fig. 4 for (NSC and HSC) at (28 and 90) days as follows , it was similar patte those obtained by (Ayden & ect -10) Fig. The relationship between Compressi fcu=1.5676 RN –18.537 ……... fcu=1.5896 RN –10.66 ……... ( Where: fcu: Concrete compressive strength (cubic) in M RN: Rebound number. , R: Coefficient of correlation. C. Relationship between Compressive Strength and UPV The pulse velocity is not related directly to compressive strength but it is agreed that concrete compressive strength increases, the pulse velocity increases large similarity behavior of the mix (A mixed and normal strength and just difference is behavior of the mix (C40, C5 and C C100), as shown in Fig.5,the results show that the relationship between compressive strength and UPV is large similarity behavior of the all mixes are increasing the UPV by the increasing compressive strength of concrete and This increment is not linear and could be presented as exponential relationship, this result is similar to result from (Ramazan, & etc From the Fig.5 below which shows that the value of UPV is affect by optimum selection of mix proportion for concrete, and increasing it because the increasing cement content and concrete homogeneity, and this properties caused decreasing poros 0 10 20 30 40 50 60 70 80 90 100 10 20 CompressiveStrength-MPa 28-day 90-day International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 11 The Fig. 3 shows that the value of RN is affect by mix proportion of concrete, and increasing it because the increasing coarse aggregate and concrete homogeneity, and this properties caused sing hardness of concrete. The Fig. 4 shows the relationship between compressive strength of for the all mixes at all ages. After using statistical analyses by (SPSS.19) program, it could be found that the linear her coefficient of correlation than other expressions, the expression obtained from Fig. 4 for (NSC and HSC) at (28 and 90) days as follows , it was similar patte 10)[28] he relationship between Compressive strength-RN at (7, 28, 56, 90) day for all mixes ……... (III -1) at [28days ,R2 =0.964] ……... (III-2) at[90days ,R2 =0.973] oncrete compressive strength (cubic) in MPa. : Coefficient of correlation. C. Relationship between Compressive Strength and UPV The pulse velocity is not related directly to compressive strength but it is agreed that concrete compressive strength increases, the pulse velocity increases[29]. Also, the results show large similarity behavior of the mix (A1, A2, A3 and A4) and (B1, B2, B3 and B4) because it is ready mixed and normal strength and just difference is with changing in (w/c) ratio, and show similarity and C60), and show similarity behavior of the mix(C ), as shown in Fig.5,the results show that the relationship between compressive strength and ge similarity behavior of the all mixes are increasing the UPV by the increasing compressive strength of concrete and This increment is not linear and could be presented as exponential relationship, this result is similar to result from (Ramazan, & etc -04) [30] From the Fig.5 below which shows that the value of UPV is affect by optimum selection of mix proportion for concrete, and increasing it because the increasing cement content and concrete homogeneity, and this properties caused decreasing porosity of concrete. fcu= 1.5676R R² = 0.9644 fcu= 1.5896R R² = 0.9732 30 40 50 60 Rebound number International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (2013), © IAEME is affect by mix proportion of concrete, and increasing it because the increasing coarse aggregate and concrete homogeneity, and this properties caused sing hardness of concrete. The Fig. 4 shows the relationship between compressive strength of After using statistical analyses by (SPSS.19) program, it could be found that the linear her coefficient of correlation than other expressions, the expression obtained from Fig. 4 for (NSC and HSC) at (28 and 90) days as follows , it was similar patteRN to at (7, 28, 56, 90) day for all mixes The pulse velocity is not related directly to compressive strength but it is agreed that as the Also, the results show ) because it is ready with changing in (w/c) ratio, and show similarity ), and show similarity behavior of the mix(C70, C80, C90 and ), as shown in Fig.5,the results show that the relationship between compressive strength and ge similarity behavior of the all mixes are increasing the UPV by the increasing compressive strength of concrete and This increment is not linear and could be presented as [30] . From the Fig.5 below which shows that the value of UPV is affect by optimum selection of mix proportion for concrete, and increasing it because the increasing cement content and concrete RN - 18.537 9644 RN - 10.66 9732 70
12.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue Fig. 5 the relationship between Compressive strength (C40, C50, C The Fig. 6 shows the relationship between compressive strength (28, 90) days. Fig.6 the relationship between Compressive strength 1:1.5:3, (C40, C The expressions which represent the relationship betw from Fig. 6 for (NSC and HSC) at (28, 90) days. 5 15 25 35 45 55 65 75 85 95 105 115 2.5 3 Compressivestrength-MPa 1:2.5:4. 0 10 20 30 40 50 60 70 80 90 100 3 3.3 3 Compressivestrength-MPa 28-day 90-day International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 12 Fig. 5 the relationship between Compressive strength-(UPV) for the all mixes (1:2:4, 1:1.5:3, , C60) and (C70, C80, C90, C100) at all ages The Fig. 6 shows the relationship between compressive strength-UPV for all mixes as Fig.6 the relationship between Compressive strength-(UPV) at all ages for the mixes (1:2:4, , C50, C60) and (C70, C80, C90, C100) at all ages The expressions which represent the relationship between compressive strength and UPV from Fig. 6 for (NSC and HSC) at (28, 90) days. 3.5 4 4.5 5 Ultrasonic Pulse Velocity-km/sec .63 1:1.91:3.5 fcu= 0.5993e0.9981 fcu = 0.4736e1 3.6 3.9 4.2 4.5 4.8 Ultrasonic pulse velocity-km/sec International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (2013), © IAEME (UPV) for the all mixes (1:2:4, 1:1.5:3, UPV for all mixes as group, for (UPV) at all ages for the mixes (1:2:4, een compressive strength and UPV 5.5 9981V 1.1035V 5.1
13.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue fcu=0.5993 e 0.9981V ……….(III-3 fcu=0.4736 e 1.10351V ……….(III-4) Where: fcu in (MPa) and V:UPV in (km/sec). D. Combined Non-destructive Tests It is advantageous to use more than one method of NDT at a time, especially when a variation in properties of concrete affects the test results in opposite direc presence of moisture in concrete: an increase in the moisture content increases the UPV, but decreases the rebound number recorded by the rebound hammer The using combination of test results of UPV and concrete. By method of multiple linear regression analysis using (SPSS.19) computer program to obtained mathematical expression, graph it by (axcel.2010), it becomes easy to obtain an expression which represents the relation between UPV and rebound number versus compressive strength. The Fig. 7, 8, 9 and 10 show for all mixes as the group at similar to the results obtained from (Raouf and Samurai expressions can be expressed as follows fcu=0.42 RN 0.63 e 0.58V ……….( fcu=0.25 RN 0.45 e 0.85V ……….(III Where: fcu in (MPa), and Fig. 7 Curves for comp. strength of concrete and combined UPV and 0 10 20 30 40 50 60 70 80 90 100 110 120 0 10 20 Compressivestrength-MPa UPV in km/sec International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 13 3) at [28days ,R2 =0.9755] ) at [90days ,R2 =0.9753] a) and V:UPV in (km/sec). destructive Tests It is advantageous to use more than one method of NDT at a time, especially when a variation in properties of concrete affects the test results in opposite directions. Such as the case with the presence of moisture in concrete: an increase in the moisture content increases the UPV, but decreases the rebound number recorded by the rebound hammer [31], [32] . The using combination of test results of UPV and RN to estimate compressive strength of concrete. By method of multiple linear regression analysis using (SPSS.19) computer program to obtained mathematical expression, graph it by (axcel.2010), it becomes easy to obtain an expression between UPV and rebound number versus compressive strength. The Fig. 7, 8, 9 and 10 show for all mixes as the group at (28 and 90) days, the results are similar to the results obtained from (Raouf and Samurai-99[14] and Qasrawi- ns can be expressed as follows: ……….(III-5) at [28days , R2 = 0.9929] III-6) at [90-days, R2 = 0.9954] and V:UPV in (km/sec). Fig. 7 Curves for comp. strength of concrete and combined UPV and RN 20 30 40 50 60 Rebound number International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (2013), © IAEME It is advantageous to use more than one method of NDT at a time, especially when a variation tions. Such as the case with the presence of moisture in concrete: an increase in the moisture content increases the UPV, but timate compressive strength of concrete. By method of multiple linear regression analysis using (SPSS.19) computer program to obtained mathematical expression, graph it by (axcel.2010), it becomes easy to obtain an expression between UPV and rebound number versus compressive strength. (28 and 90) days, the results are -2000[33] ). The at 28 days 70
14.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue Fig. 8 Comparison of predicted comp. strength with measured comp. strength of concrete at Fig. 9 Curves for comp. streng 0 10 20 30 40 50 60 70 80 90 100 110 120 130 0 10 20 Compressivestrength-MPa UPV in km/sec Predicted vs. Observed values f ObserveddataMPa International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 14 Fig. 8 Comparison of predicted comp. strength with measured comp. strength of concrete at age 28 days Fig. 9 Curves for comp. strength of concrete and combined UPV and RN 20 30 40 50 60 Rebound number Predicted vs. Observed values – 28 day f R0.63 * exp(0.58*V) International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (2013), © IAEME Fig. 8 Comparison of predicted comp. strength with measured comp. strength of concrete at at 90 days 70
15.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue Fig. 10 Comparison of predicted comp. strength with measured comp. strength of concrete at Fig. 11 and 12 show for all mixes as the group and for all ages, the results are similar to the results obtained from (Raouf and Samurai fcu=0.44 RN 0.65 e 0.55V ……….(III Where: Fig. 11 Curves for comp. strength of concrete and combined UPV and 0 20 40 60 80 100 120 0 10 Compressivestrength-MPa UPV in km/sec Predicted vs. Observed values ObservedvaluesMPa International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 15 Fig. 10 Comparison of predicted comp. strength with measured comp. strength of concrete at age 90 days Fig. 11 and 12 show for all mixes as the group and for all ages, the results are similar to the results obtained from (Raouf and Samurai-99)[14]. The expressions can be expressed, as follows: III-7) at[All ages R2 = 0.9729] Where: fcu in (MPa) and V:UPV in (km/sec). for comp. strength of concrete and combined UPV and RN 20 30 40 50 60 Rebound number Predicted vs. Observed values – 90 day fcu= 0.25* R0.45 * exp (0.85*V) International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (2013), © IAEME Fig. 10 Comparison of predicted comp. strength with measured comp. strength of concrete at Fig. 11 and 12 show for all mixes as the group and for all ages, the results are similar to The expressions can be expressed, as follows: at (all ages) 70
16.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue Fig. 12 Comparison of predicted comp. strength with measured comp. strength of concrete at E. Relationship between direct (D) and surfacing (S) test of UPV Indirect transmission should be used when only one face of the concrete is the depth of a surface crack is to be determined or when the quality of the surface the overall quality is of interest. Furthermore, which are usually influenced by the concrete composition from that of the concrete within unrepresentative of that concrete. The the same concrete element. This difference may vary from 5% to 20% depending largely on the quality of the concrete under test [10], is shown in Fig. 13, 14, 15 and 16. The Figures show that the waves velocity of surfacing method less than the waves velocity of direct method by (7, 5 and 3.5)% at (7, 28and 90) days respectively because the porosity of concrete that is near the surface more than the porosity of deep concrete Fig. 13 Relationship between 0 10 20 30 40 50 60 70 80 2.5 3 Compressivestrength-MPa 7-direct 7-surfacing Predicted vs. Obser fObservedvaluesMPa International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 16 Fig. 12 Comparison of predicted comp. strength with measured comp. strength of concrete at all ages E. Relationship between direct (D) and surfacing (S) test of UPV nsmission should be used when only one face of the concrete is the depth of a surface crack is to be determined or when the quality of the surface concrete relative to the overall quality is of interest. Furthermore, this arrangement gives pulse velocity measurements which are usually influenced by the concrete near the surface. This region is often of different composition from that of the concrete within the body of a unit and the test results may be unrepresentative of that concrete. The indirect velocity is invariably lower than the direct velocity on difference may vary from 5% to 20% depending largely on the [10], the relationship between direct and surfacing method of The Figures show that the waves velocity of surfacing method less than the waves velocity of direct method by (7, 5 and 3.5)% at (7, 28and 90) days respectively because the porosity of concrete urface more than the porosity of deep concrete [10] [34] . Fig. 13 Relationship between direct and surfacing method of UPV at 7 days all mixes 3.5 4 4.5 Ultrasonic Pulse Velocity-km/sec Predicted vs. Observed values – at all age fcu = 0.44* R 0.65 * exp (0.55*V) International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (2013), © IAEME Fig. 12 Comparison of predicted comp. strength with measured comp. strength of concrete at accessible, when concrete relative to pulse velocity measurements near the surface. This region is often of different the body of a unit and the test results may be velocity is invariably lower than the direct velocity on difference may vary from 5% to 20% depending largely on the the relationship between direct and surfacing method of UPV The Figures show that the waves velocity of surfacing method less than the waves velocity of direct method by (7, 5 and 3.5)% at (7, 28and 90) days respectively because the porosity of concrete direct and surfacing method of UPV at 7 days all mixes 5 km/sec
17.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue Fig. 14 Relationship between direct and surfacing method of UPV at 28 day all mixes Fig. 15 Relationship between V. CONCLUSIONS 1- Concretes with compressive strengths in excess of 60 N/mm SF. 2- High early compressive strength (in excess of 25 N/mm 3- Linear expressions are obtained to represent the relationship between density and UPV for (28 and 90) days respectively, as follows: D = 134.98(V)+1814.8 .........(V D = 159.45(V)+1680.1 .........(V 0 10 20 30 40 50 60 70 80 90 100 3 3.2 3.4 Compressivestrength-MPa 28-direct 28-surfacing 0 10 20 30 40 50 60 70 80 90 100 3.25 3.45 3.65 Compressivestrength-MPa 90-direct 90-surfacing International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 17 direct and surfacing method of UPV at 28 day all mixes direct and surfacing method of UPV at 90 day all mixes compressive strengths in excess of 60 N/mm2 are more easily achieved with High early compressive strength (in excess of 25 N/mm2 at 24 hours) can be ac Linear expressions are obtained to represent the relationship between density and UPV for (28 90) days respectively, as follows: .........(V-1) [28-day, R2 = 0.9287] .........(V-2) [90-day, R2 = 0.8751] 3.6 3.8 4 4.2 4.4 4.6 Ultrasonic Pulse Velocity-km/sec 3.85 4.05 4.25 4.45 4.65 4.85 Ultrasonic Pulse Velocity-km/sec International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (2013), © IAEME direct and surfacing method of UPV at 28 day all mixes direct and surfacing method of UPV at 90 day all mixes easily achieved with at 24 hours) can be achieved. Linear expressions are obtained to represent the relationship between density and UPV for (28 4.8 km/sec 5.05
18.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 18 4- The results show a good correlation between compressive strength and rebound number and the relationship between the two is not affected by maximum aggregate size (MAS) 5- Linear expressions are obtained to represent the relationship between compressive strength and RN for all mixes as group for (28 and 90) days respectively, as follows: fcu = 1.5676 RN - 18.537 .........(V-3) [28-day, R2 = 0.964] fcu = 1.5896 RN - 10.66 .........(V-4) [90-day, R2 = 0.973] 6- The value of UPV in HSC increased 8% from (28 to 90) days because of using SF. 7- Exponential expressions are obtained to represent the relationship between compressive strength and UPV for 28 and 90days respectively, as follows: fcu = 0.5993 e 0.9981 V .........(V-5) [28-day, R2 = 0.9755] fcu = 0.4736 e 1.1035 V .........(V-6) [90-day, R2 = 0.9753] 8- The results indicate that the percentage of increase in direct method to surfacing method of UPV for (7, 28, 56 and 90) days are (7%, 5%, 4% and 3.5%) respectively, due to the higher the continuity of hydration of cement. 9- The combined use of UPV and rebound number improves the accuracy of the process of estimation of concrete compressive strength of (HSC). 10- The results show that the relation between UPV and RN versus compressive strength, can be expressed for all the mix as a case freelance for all ages, as follows: fcu = 0.37 RN 0.75 e 0.5V .........(V-7) [all ages, R2 = 0.9908] for (1:2:4) fcu = 0.172 RN 0.7 e 0.75V .........(V-8 ) [all ages, R2 = 0.994] for (1:1.5:3) fcu = 0.15 RN 0.47 e 0.95V .........(V-9) [all ages, R2 = 0.8416] for (C40, C50 and C60) fcu = 0.18 RN 1.33 e 0.17V .....(V-10) [all ages, R2 = 0.962] for (C70, C80, C90 and C100) 11- The results show that the relation between UPV and rebound number versus compressive strength, can be expressed for all the mix as group, for (28 and 90) days, as follows: fcu = 0.42 RN 0.63 e 0.58V .........(V-11) [28-days, R2 = 0.9929] fcu = 0.25 RN 0.45 e 0.85V .........(V-12) [90-days, R2 = 0.9954] 12- The results show that the relation between UPV and rebound number versus compressive strength, can be expressed for all the mix as group, for all ages, as follows: fcu = 0.44 RN 0.65 e 0.55V .........(V-13) [all ages, R2 = 0.9729] 13- The pulse velocity of concrete is decreased by increasing the cement paste, especially for concrete with high w/c. 14- The increasing of cement content gives increasing in value of UPV but not exceeded (500 kg/m3). 15- Rebound number can't be affected by changing MAS of coarse aggregate. 16- The increasing of coarse aggregate content produces increasing the value of RN and UPV. VI. REFERENCES [1] J.Balsam,“Properties and Testing of Concrete Materials” Al- Tahhadi University, Engineering College, Libya, 2008, pp. 2-5. [2] ACI committee 211.1, 2002, “Standard practice for selecting proportions for normal, heavyweight, and mass concrete,” American Concrete Institute. [3] ACI committee 318M, 2005, “Building code requirements for structural concrete and commentary,” American Concrete Institute. [4] ACI committee 363R, 1997, “State of the art report on high-strength concrete,” American Concrete Institute. Detroit, Vol. 81, No.4. [5] H. G. Russell, “High-performance concrete mix proportions,” Concrete Products Magazine, Issue. June, 2000.
19.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 19 [6] B.Price, “high strength concrete,” advanced concrete technology set, part III, Elsevier, chapter 3, 2003, pp. 1-16. [7] M. A.Caldarone, “High-strength concrete: A practical guide” Taylor and Francis, USA and Canada,2008. [8] ACI Committtee 228.1R-95, “In-Place Methods to Estimate Concrete Strength”, American Concrete Institute, Detroite, 1995. [9] N.J.Carino, “Nondestructive Testing of concrete: History and Challenges”, SP 144-30, American Concrete Institute, Detroite, 1994 , pp.623-678. [10] IAEA: InteRNational Atomic Energy Agency, “Guidebook on Non-destructive testing of concrete structures”, Vienna, 2002, pp.1-2. [11] A.Hussam, “Non-destructive Tests For Self-Compacting Concrete With Compressive Strength In Range (20-80)Mpa” Master Thesis, L-Mustansiriya , January 2008. [12] J.Kolek , “Nondestructive testing of concrete by hardness methods”, Symposium on Non- destructive testing of concrete and tember, The Institution of Civil Engineers, (London, 1970) pp.19-22. [13] V.M. Malhotra & N.J. Carino, “Handbook On Non-destructive Testing of Concrete” Boca Raton London New York Washington, D.C.,(pp.19-29), (pp.189-204) and (pp.209-213). [14] Z.A. Raouf &M. Samurai, “Nondestructive testing of concrete” Edition No. 1, Shariga,1999. [15] Iraqi Specification, No.5/1984, “Portland cement,” Central Organization Standardization& Quality Control(C.O.S.Q.C.) , Baghdad. [16] Iraqi Specification, No.45/1984, “Aggregates from natural sources for concrete and construction,” Central Organization Standardization& Quality Control(C.O.S.Q.C.) , Baghdad. [17] American Society for Testing and Materials, ASTM C1240-2005, “Standard Specification for Use of Silica Fume as a Mineral Admixture in Hydraulic Cement Concrete, Mortar, and Grout,” Annual Book of ASTM Standards, Vol. 15-02. [18] Iraqi Specification, No.1431/1988, “concrete admixtures,” Central Organization Standardization& Quality Control (C.O.S.Q.C.) , Baghdad. [19] American Society for Testing and Materials, ASTM C 494 -2005, “Standard specification for chemical admixtures for concrete,” Annual Book of ASTM Standards, Vol. 04-02. [20] ACI Committee 212.4R, 2004, “Guide for the use of high-range water-reducing admixtures (superplasticizers) in concrete,” American Concrete Institute. [21] ACI committee 211.1, 2002, “Standard practice for selecting proportions for normal, heavyweight, and mass concrete,” American Concrete Institute. [22] T. C. Holland, “Silica Fume User’s Manual,” first edition, Federal Highway Administration, Washington, 193 pp, 2005 [23] D. Hekmat,“ Mix design for high strength concrete with silica fume”, Master Thesis, Babylon University, July- 2010. [24] Iraqi Specification, No.354/1990, “Determination of slump,” Central Organization Standardization& Quality Control(C.O.S.Q.C.) , Baghdad. [25] Iraqi Specification, No.325/1993, “Determination Rebound number of concrete,” Central Organization Standardization& Quality Control (C.O.S.Q.C.) , Baghdad. [26] Iraqi Specification, No.300/1991, “Pulse velosity through concrete” Central Organization Standardization& Quality Control(C.O.S.Q.C.) , Baghdad. [27] Iraqi Specification, No.284/1991, “compression testing machines for concrete,” Central Organization Standardization& Quality Control (C.O.S.Q.C.), Baghdad. [28] F. Aydin & M. Saribiyik “Correlation between Schmidt Hammer and destructive compressions testing for concretes in existing buildings” Scientific Research and Essays Vol. 5(13), p.p. 1644-1648,4 July 2010.
20.
International Journal of Civil Engineering and Technology (IJCIET), ISSN 0976 – 6308 (Print), ISSN 0976 – 6316(Online) Volume 4, Issue 4, July-August (2013), © IAEME 20 [29] G. Trtnik& F. Kavcˇic & G. Turk “Prediction of concrete strength using ultrasonic pulse velocity and artificial neural networks” available at Science Direct Elsevier Ultrasonic (49) May (2008) p.p. 53-60. [30] R. Demirbog, I. Tu¨rkmen & M. B. Karakoc “Relationship between ultrasonic velocity and compressive strength for high-volume mineral-admixtured concrete” Cement and Concrete Research (34) p.p. 2329–2336, 15 April 2004. [31] Neville, A.M., “Properties of Concrete”, Fifth Edition, Pitman Press, London, United Kingdom, 1995, pp.261-264. [32] H.Y. Qasrawi, “Concrete strength by combined nondestructive methods Simply and reliably predicted” Cement and Concrete Research(30),p.p. 739-746 ,28 January 2000. [33] H.Y. Qasrawi “Concrete strength by combined nondestructive methods simply and reliably predicted (discussion)” Cement and Concrete Research (31), October 2000(pp.1239-1240). [34] J.H.Bungey& S.G. Millard, “Testing of Concrete in Structures”, Third Edition, United Kingdom, Glasgow, pp. 50, 1996. [35] Alaa Abdul Kareem Ahmad, “The Effect of Gypsum Compensative on Mortar Compressive Strength”, International Journal of Civil Engineering & Technology (IJCIET), Volume 4, Issue 3, 2013, pp. 168 - 175, ISSN Print: 0976 – 6308, ISSN Online: 0976 – 6316. [36] Dr. Tareq S. Al-Attar, “A Mathematical Model for Predicting Autoclave Expansion for Portland Cement”, International Journal of Civil Engineering & Technology (IJCIET), Volume 4, Issue 1, 2013, pp. 110 - 116, ISSN Print: 0976 – 6308, ISSN Online: 0976 – 6316. [37] Vinod P, Lalumangal and Jeenu G, “Durability Studies on High Strength High Performance Concrete”, International Journal of Civil Engineering & Technology (IJCIET), Volume 4, Issue 1, 2013, pp. 16 - 25, ISSN Print: 0976 – 6308, ISSN Online: 0976 – 6316. [38] P.J.Patel, Mukesh A. Patel and Dr. H.S. Patel, “Effect of Coarse Aggregate Characteristics on Strength Properties of High Performance Concrete using Mineral and Chemical Admixtures”, International Journal of Civil Engineering & Technology (IJCIET), Volume 4, Issue 2, 2013, pp. 89 - 95, ISSN Print: 0976 – 6308, ISSN Online: 0976 – 6316.
×
Share Painel de recortes
×
Email
Email sent successfully..
Facebook
Twitter
LinkedIn
Google+
Link
Be the first to comment